OSWAGO MOSES OWINO (B.ED. Sc.) I56/CE/12222/2007
A THESIS SUBMITTED IN PARTIAL FULFILLMENT OF THE REQUIREMENTS FOR THE AWARD OF THE DEGREE OF MASTER OF
SCIENCE (CHEMISTRY) IN THE SCHOOL OF PURE AND APPLIED SCIENCES OF KENYATTA UNIVERSITY
I declare that this thesis is my original work and has not been presented for a degree in any other university or any other award
Signature ………. Date ……….. Oswago Moses Owino (I56/12222/2007)
Department of Chemistry
We confirm that the work reported in this thesis was carried out by the candidate under our supervision
Signature ………. Date ……… Prof. Naftali T. Muriithi
Department of Chemistry Kenyatta University
Signature ………. Date ……… Dr. Harun M. Mbuvi
I would like to thank the Almighty God for life, wisdom and resources.
My gratitude goes to the academic and technical staff and post graduate students of Chemistry department from Kenyatta University for constructive critique and corrective interactions which directed the work to successful completion. My sincere thanks go to my supervisors, the late Prof. Naftali Muriithi (May his soul rest in eternal peace) and Dr. Harun Mbuvi whose academic ingenuity, professional guidance and resource support pushed the work to a successful end.
TABLE OF CONTENTS
DECLARATION ... ii
DEDICATION ... iii
ACKNOWLEDGEMENTS ... iv
LIST OF TABLES ... ix
LIST OF APPENDICES ... x
ABBREVIATION AND ACRONYMS ... xi
ABSTRACT ... xii
CHAPTER ONE ... 1
INTRODUCTION ... 1
1.1BACKGROUND INFORMATION ... 1
1.3JUSTIFICATION OF THE STUDY ... 5
1.4OBJECTIVES ... 6
1.5THE SCOPE OF STUDY ... 6
1.6LIMITATIONS OF THE STUDY ... 7
CHAPTER TWO ... 8
LITERATURE REVIEW ... 8
2.1DEFINITION OF CLAY AND CLAY MINERALS ... 8
2.2PROPERTIES OF CLAYS ... 9
2.3 OCCURRENCE OF THE CLAY MINERALS ... 13
2.5INFLUENCE OF INORGANIC ACIDS ON CLAYS ... 25
2.6CLAY AS A POSSIBLE RAW MATERIAL FOR CERAMICS ... 26
2.7CLAY AS A SOURCE OF ALUMINIUM ... 26
2.7EFFECT OF IMPURITIES ON PROPERTIES OF CLAY ... 27
2.8USES AND APPLICATIONS OF CLAY AND ITS MINERALS ... 30
2.9ANALYTICAL METHODS/INSTRUMENTS ... 34
184.108.40.206INSTRUMENTATION OF AAS ... 35
220.127.116.11PRINCIPLE OF XRD ... 36
18.104.22.168INSTRUMENTATION AND WORKING OF XRD ... 37
22.214.171.124PRINCIPLE OF INFRARED SPECTROSCOPY (IR) ... 40
126.96.36.199 INSTRUMENTATION IN IR ... 41
CHAPTER THREE ... 43
MATERIALS AND METHODS ... 43
3.1THE STUDY AREA. ... 43
3.2APPARATUS,CHEMICALS AND MATERIALS ... 46
3.3SAMPLE PRE-TREATMENT AND ANALYSIS ... 49
188.8.131.52PREPARATION OF 0.05MEDTASOLUTION... 50
184.108.40.206PREPARATION OF SOLOCHROME BLACK INDICATOR ... 51
220.127.116.11PREPARATION OF 0.01MZINC SULPHATE SOLUTION ... 51
18.104.22.168PREPARATION OF STANDARD 0.05MFE3+SOLUTION ... 51
22.214.171.124DETERMINATION OF FE3+IN CLAY SAMPLES BY EDTA TITRATION ... 52
126.96.36.199DETERMINATION OF AL3+IN CLAY SAMPLES BY EDTATITRATION ... 52
3.4X-RAY FLUORESCENCE SPECTROPHOTOMETER (XRFS)ANALYSIS ... 53
3.5X-RAY DIFFRACTION (XRD)ANALYSIS ... 53
3.6INFRARED (IR)ANALYSIS ... 55
3.7LEACHING THE CLAYS WITH MINERAL ACIDS AT ROOM AND BOILINGTEMPERATURES………..57
3.8LOSS ON IGNITION (LOI) ... 58
CHAPTER FOUR ... 59
RESULTS AND DISCUSSION ... 59
4.2CHEMICAL ANALYSIS OF RAW CLAYS IN THE STUDY KANO PLAINS ... 59
4.3MINERAL ANALYSIS OF RAW CLAYS ... 64
4.4CHEMICAL ANALYSIS OF ACID-TREATED CLAYS ... 71
4.5MINERAL ANALYSIS OF ACID-TREATED CLAYS ... 76
CHAPTER FIVE ... 82
CONCLUSIONSANDRECOMMENDATIONSFORFURTHERSTUDIES ... 82
5.2CONCLUSIONS ... 82
5.3RECOMMENDATIONS ... 83
REFERENCES ... 85
APPENDIX 1 ... 92
Tables of Detailed Elemental Analysis Results of Raw Clays ...92
APPENDIX 2 ... 99
Graphs of Additional Data ... 99
APPENDIX 3 ... 104
Summary of Minerals Detected In Raw and Acid-Treated Clays ... 104
APPENDIX 4 ... 105
IR ANALYSIS SPECTRA ... 105
APPENDIX 5 ... 107
LIST OF FIGURES
Figure 2.1. Silica tetrahedral layers……….18
Figure 2.2. Alumina-octahedron layer………....…….18
Figure2.3. Coordination of cation, T, and oxygen atoms, O, in a tetrahedron…………19
Figure 2.4. The Octahedron and the octahedral sheet………..20
Figure 2.5. Models of a 1:1 and 2:1 layer structure...22
Figure 2.6. (a) Tri-octahedral sheet; (b) Di-octahedral sheet...23
Figure 2.7. The octahedral sites...24
Figure 2.8. Views of 1:1 and 2:1 layer from x-axis (A) and y-axis (B)...24
Figure 2.9. Silicate layer: 1:1 and 2:1 structures...25
Figure 2.10 Schematic of an atom, depicting energy transitions……….38
Figure 3.1 Map of Kano Plains, Kisumu County, Kenya………43
Figure 3.2 Soil survey map for Kano Plains, Kenya………..……..44
Figure 4.1(a): XRD analysis of raw clay sample from sample 3076...66
Figure 4.1(b): XRD analysis of raw clay sample from composite sample ...67
Figure 4.2(a) IR spectrum of clay sample from sample 3076………..70
Figure 4.2(b) IR spectrum of clay sample from sample 3078………..71
Figure 4.3(a): XRD analysis of acid-boiled clay sample from sample 3076...79
LIST OF TABLES
Table 3.1 Sampling sites and Indexing...……… 43
Table 3.2 Percentage mineral composition of rock standards………. 44
Table 3.3 Instrumental conditions and settings for AAS analysis………45
Table 3.4 XRF voltage and current settings for analysis of elements in clay samples……….45
Table 3.5 Major d-spacings for some minerals that occur in soils………..52
Table 3.6 IR Identification peaks for clay minerals……….54
Table 4.1 Full Assay analysis of clays from Kano Plains by AAS………..59
Table 4.2 Ranges of percentage elemental composition………...60
Table 4.3 Percentage mean composition of different minerals ………61
Table 4.4 The IR peaks identified………...66
Table 4.5 Boiling temperature of Acid-clay mixtures for HCl and H2SO4...67
Table 4.6 Percentage SiO2, Al2O3 and Fe2O3 in HCl-treated clays...68
Table 4.7(a) Summary of average percentage Fe2O3 in raw and acid-treated clays...72
Table 4.7(b) Summary of average percentage Al2O3 in raw and acid-treated clays...72
Table 4.8(a) Minerals and % composition in raw and acid-boiled clay samples...78
LIST OF APPENDICES
Tables of Detailed Elemental Analysis Results of Raw Clays...92
Table 6.1 Full assay results from AAS, XRF and EDTA for raw clays...92
Table 6.2 Full assay AAS analysis of raw clays ………...93
Table 6.3 Mean Percentage Composition of Different Minerals ………...94
Table 6.4 Percentage Fe2O3 in raw and H2SO4 - treated clay samples ...95
Table 6.5 Percentage Fe2O3 in different concentrations of HCl and H2SO4...96
Table 6.6 Percentage Fe2O3 in raw and HCl-treated clays...97
Table 6.7 Percentage Al2O3 in raw and HCl-treated clays...98
Graph 6.1 Fe2O3 in each raw clay samples...99
Graph 6.2 Percentage Fe2O3 in Raw and HCl-treated Clays...100
Graph 6.3: Percentage Alumina in raw clays by different analytical methods...101
Graph 6.4: Comparison of average % Al2O3 in HCl and H2SO4-treated clays...102
Graph 6.5: Percentage aluminium oxide in HCl-treated clays...103
Summary of minerals detected in raw and acid-treated clays……….……..104
Table 6.8 Percentage compositions of clay minerals raw clays in one ...104
IR ANALYSIS SPECTRA...105
Spectrum 6.1 IRS spectrum for clay sample from Riat Market, Kano Plains, Kenya...105
Spectrum 6.2 IR spectrum for clay sample from Anywang’, Kano Plains, Kenya...106
APPENDIX 5………. ………..107
ABBREVIATION AND ACRONYMS
AAS –Atomic Absorption Spectrometry ANOVA- Analysis of Variance
CCMET- Canadian Centre for Mineral and Energy Technology EDS- Energy Dispersive System
EDTA- Ethylenediaminetetraacetic Acid
ICRAF- International Centre of Research in Agriculture and Forestry IR- Infra-Red Spectroscopy
JKUAT- Jomo Kenyatta University of Agriculture and Technology KNBS- Kenya National Bureau of Statistics
LOI – Loss of Ignition
NIB- National Irrigation Board
SPSS- Statistical Package for the Social Sciences WDS- Wavelength Dispersive System
INTRODUCTION 1.1 Background Information
Clay soils have mineral groups like kaolinite, smectites, illites and palygorskite-sepiolite (Murray, 2004) with unique properties and industrial and economic uses other than farming. Other uses include manufacture of cement, making bricks and floor tiles, additive in medicinal ointments, catalyst in cracking reactions, manufacture of drilling clays, making lead pencils, fillers in paper industry, use in printing inks, and use in paints and making ceramic products (Murray, 2004).
Clay minerals are hydrous aluminosilicates with phyllosilicate structure and with very small-grained particles of less than 4µm (Mason, 1968). The classes of clay minerals includes smectites (montmorillonite, saponite), mica (illite), kaolinite, serpentine, pylophyllite (talc), vermiculite and sepiolite (Shichi and Takagi, 2000). Clays have adsorption capabilities which result from a net negative charge on the structure of minerals and sorption properties attributed to their high surface area and high porosity (Alkan et al., 2004).
packed oxygens and hydroxyls in which aluminium, iron and magnesium atoms are embedded in an octahedral combination so that they are equidistant from six oxygens or hydroxyls. The second unit is built of silica tetrahedrons arranged to form a hexagonal network that is repeated indefinitely to form a sheet of composition, Si4O6(OH)4 hydrated aluminium silicates with very fine particle size, usually <2mm (Ralph, 1968). A layered structure is formed by the tetrahedral sheet(s) linked to octahedral sheet through sharing of apical oxygens. The tetrahedra contain mainly Si(IV) as the central atom, while the octahedral sites are occupied mostly by Al(III), Fe(III) or Mg(II). If one tetrahedral and one octahedral sheet are bonded together the structure is called 1:1 layer silicate structure. The structure created from two tetrahedral sheets sandwiching an octahedral sheet is called 2:1 layer silicate.
Kano plains are located in the western part of Kenya, Kisumu County and cover the sub-counties of Nyando, Nyakach and Kisumu East. The soils are fine-grained black and grey coloured, become plastic when wet and later become hard and form cracks during dry season. The soils are poorly drained and aerated when wet. The clays in the region are currently used for subsistence farming on a small scale and rice production under National Irrigation Board (NIB) on a large scale. The subsistence farming has frequent failures due to unreliable rainfall and floods that are most prevalent in March to May of each year.
Clays are classified into earthenware clay, mid-fire stoneware clay and high-fire stoneware clay depending on the temperature at which they are fired to reach maximum hardness (Barsoum, 2003). They can be modified to make ceramic matrix composite materials with superior characteristics than either of the components (Chawla, 1993). The practical effectiveness of several organic acids such as acetic, formic, citric and ascorbic acids used for dissolving iron from iron compounds have also been evaluated (Ambikadevi and Lalithambika, 2000). Oxalic acid was found to be the most promising because of its acid strength, good complexing characteristics and high reducing power, compared to other organic acids.
Rural water Supply and Sanitation program (MLA Engineers, 1988) and The Soils of Nyando Catchment Area – Reconnaissance Soil Survey Report (Waruru et al., 2003). These studies have addressed the area as a whole with respect to natural catastrophes (floods and drought), improvement of water resources and sanitation and general soil survey. Other possible uses of clays like making Portland cement, floor tiles, high quality ceramics would be revealed if the chemical and mineral composition of the clays were known. However, such studies have not been done in Kano Plains’ soils. The chemical and mineral composition of the clays explains properties which in turn determine industrial and other economic uses of the clays. Such have not been done on the clays yet its findings would reveal other alternative uses of the clays other than the current main use of rice production and subsistence farming as the only major economic uses.
whether the level of iron can be minimised to a level which would render the clays high quality raw materials for manufacture of high quality ceramic products.
1.3 Justification of the Study
Clay contains many elements and minerals in different proportions which determine its ultimate properties and uses (Grimshaw, 1971). Clays are raw materials for ceramics but have impurities like organic matter, iron and other metal oxides that could be removed by use of distilled water, organic and mineral acids, magnetic separators and froth flotation to improve its ceramic quality (Norton, 1974 a; Reed, 1988; Richerson, 1992).
iron, if any, from the clays using minerals acids so as to boost use of the clays as raw materials for high quality ceramics. The findings will relieve Kenya of cost of importing clays and help improve the economy.
1.4.1 General objective
To determine elemental composition and identify clay minerals in raw and acid-treated clays from Kano plains, Kenya.
1.4.2 Specific objectives
i) To determine the percentage composition of SiO2, Al2O3, Fe2O3, MgO, K2O, Na2O, MnO, CaO, TiO2 and water in the clays using AAS, XRF, EDTA titrations and LOI ii) To determine the percentage composition of SiO2, Al2O3 and Fe2O3 in acid-treated clays iii) To identify the clay minerals in raw and acid-boiled clay soils of Kano plains using
XRD and IR
1.5 The Scope of Study
1.6 Limitations of the Study
LITERATURE REVIEW 2.1 Definition of Clay and Clay Minerals
crystalline in nature with layer silicates formed by condensation of sheets of linked Si(OH)4 tetrahedra with those of linked M2-3(OH)6 octahedra, as the basic structure (M is either a divalent or trivalent cation) (Theng, 1974). The grains are plate-shaped and slide over each others’ surface thereby contributing to the smooth feel. They contain impurities that contribute to plasticity, melt and colour (Zakin, 2001).
2.2 Properties of Clays
Clays have very fine particles that yield very large-specific surface areas that are physically sorptive and chemically surface-active. Many clay minerals carry excess negative electric charge owing to internal substitution of Si+4 by lower valent cations and thereby increase internal chemical reactivity in chemical combination and ion exchange. These characteristics contribute to the properties of clays which are of technical applications (Murray, 2004).
enhanced by the presence of fine particles in the clays (Zakin, 2001). The plasticity is determined by the following;
i) Water of plasticity- the amount of water necessary to develop optimum plasticity or the range of water content in which plasticity is demonstrated.
ii) The amount of penetration of an object into the formed plastic mass of clay which is frequently done by use of a needle or some special plunger
iii) The stress necessary to deform the clay and the maximum deformation the clay will undergo before rapture at different moisture contents and with varying degrees of stress application (Murray, 2004).
adsorbed water. It is reduced by large amounts of non-clay mineral components. It increases with a decrease in particle size and presence of organic materials in some clay. It is generally higher when Na is the adsorbed cation (Murray, 1979). It is also dependent on the proportion of fine particles present such that the larger the proportion, the greater the dry strength. Other factors that affect dry strength are the degree of hydration of the colloidal fraction, the method of forming the ware and the extent of drying (McGraw-Hill, 1992).
This is the loss in volume in clay when it dries or when it is fired. There is thus both drying and firing shrinkage. Drying shrinkage is dependent on the water content, the character of clay minerals and the particle size of the constituents. It is high in very plastic clays and produce cracking and warping, and low in sandy clays or clays with low plasticity and tends to produce weak porous body. Firing shrinkage depends on the volatile materials present, the types of crystalline phase changes that take place during firing, and the dehydration characteristics of the clay minerals (McGraw-Hill, 1992)
product. Vitrification range refers to the temperature range over which the fusion of the material takes place. Some clay minerals like montmorillonites, illites and chlorites have short vitrification ranges while others like kaolinites have long vitrification ranges. Vitrification temperatures are lowered by some nonclay impurities like calcite and feldspar which act as fluxes. The degree of vitrification depends on the duration of firing as well as the temperature attained (McGraw-Hill, 1992).
2.2.6 Firing Properties
Firing property refers to the fusion and hardening of clays when heated to higher temperatures. Heating clay materials to successive higher temperatures causes fusion. Shrinkage and loss of pore waters occur in the range of 100-105 oC with attendant dimensional changes. Oxidation of sulphides present in the clays begins in temperatures of between 400-500 oC, and loss of hydroxyl waters from clay minerals takes place at between 500-900 oC. The loss of hydroxyl water is usually accompanied by a modification of the structure but not complete destruction of clay minerals. It causes shrinkage in the two layer minerals (Kaolinites and halloysites) but not in the three layer minerals (Murray, 1979). The structure of a clay mineral is destroyed in the temperature range of 800-950 oC and major firing shrinkage develops. At temperatures above 900 oC, new crystalline phases develop in all the clay minerals except those containing large amounts of Fe, alkalis, alkaline earths, for which case fusion may result after the loss of structure without any intervening crystalline phase.
2.3 Occurrence of the Clay Minerals
concentration of the mineral or a mixture of clay minerals. The four major mineral groups with different chemical and mineral composition, physical structures, and crystal orientations include kaolins, smectites (or montmorillonites), illites, and palygorskite-sepiolite groups which occur in relatively pure concentrations (Hans and Andrei, 2004). Other mineral groups are chlorites and vermiculites which occur as mixtures with non-clay minerals such as shales (Murray, 2004).
2.3.1 The Kaolin Group
Kaolin is one of the widely used clay materials for a large number of applications such as in ceramics, paper coating, paper filling, paint extender, rubber filler, cracking catalyst or cements, oil refinery and water treatment (Belver et al., 2002; Caulcante et al., 2005;Vaga, 2007; Salawudeen, 2007), cracking catalyst in the petroleum industry, use in water and oil-based paints, pencil heads, carrier of fertilizers, desiccants, and insecticides, among others (Murray, 2004). The percentage uses of kaolin in some of the technological industries are: paper filling and coating 45%; refractories and ceramic 31%, fiberglass 6%; cement 6%, rubber and plastic 5%, paint 3%, others 4% (Murray, 2002).
2.3.2 The Smectites
2.3.3 Palygorskite and Sepiolite Groups
These are hydrated magnesium aluminium silicates that have an elongated shape. They have a large surface area, and are sometimes referred to as sorptive clays, also called Fuller’s earth (Murray, 2004). The two groups are very similar but sepiolite has higher magnesium content while Palygorskite has higher aluminum content. They also have different crystal structures with palygorskite having a chain-like crystalline structure consisting of inverted ribbons of silica tetrahedron linked together by aluminium and magnesium octahedral to form a 2:1 layer structure. Some of the industrial uses of the palygorskite-sepiolite minerals include making oil-well drilling fluids that help in removing rock cuttings from the hole, making adhesives in production of corrugated paper, and making liquid suspension fertilizers among others.
2.3.4 Common Clay Group
This group includes a variety of clays and shales that are fine in particle size. The mineral composition is mixed, with illites and chlorites making the major mineral components. Illites are hydrated K, Fe- aluminium silicates while chlorites are hydrated magnesium iron aluminium silicate. Common clays are used in many structural clay products such as brick, tile, pottery, stoneware, among others (Murray,1994).
2.4 Structure and Composition of Clay Mineral
tetrahedral linked by sharing of three of the four oxygens to form sheets of pseudohexagonal network (Mason, 1968). Clay minerals are sheet structures basically composed of fine grains of silica- tetrahedral layers and alumina octahedron layers (Figures 2.1 and 2.2)
Figure 2.1. Silica tetrahedral layers, (Encyclopaedia Britannica, 1998)
Figure2.3. Coordination of cation, T, and oxygen atoms, O, in a tetrahedron and a tetrahedral sheet (a) Tetrahedron [TO4]; (b) tetrahedral sheet. Oa and Ob refer to apical and basal oxygen atoms, respectively. a and b refer to unit-cell parameters (Encyclopaedia Britannica, 1998).
Figure 2.4. The Octahedron and the octahedral sheet (a) Ooct (OH, F, Cl) orientation in cis-octahedron and trans-cis-octahedron; (b) location of cis- and trans-sites in the octahedral sheet. Oa and Ob refer to apical and basal oxygen atoms, respectively. a and b refer to unit cell parameters (Encyclopaedia Britannica, 1998).
point to the same side of the sheet and connect the tetrahedral and octahedral sheets to form a
common plane with octahedral anionic position Ooct (Ooct ¼ OH, F, Cl, O) (Figure 4). Ooct anions lie near to the centre of each tetrahedral 6-fold ring, but are not shared with tetrahedra. The 1:1 layer structure consists of the repetition of one tetrahedral and one octahedral sheet, while in the 2:1 layer structure one octahedral sheet is sandwiched between two tetrahedral sheets (Figure 2.5).
In the 1:1 layer structure, the unit cell includes six octahedral sites with four cis- and two trans-oriented octahedral and four tetrahedral sites. Six octahedral sites and eight tetrahedral sites characterize the 2:1 layer unit cell. Structures with all the six octahedral sites occupied are known as trio-octahedral (Figure 6a). If only four of the six octahedra are occupied, the structure is referred to as dioctahedral (Figure 6b).
Figure 2.6. (a) Tri-octahedral sheet; (b) Di-octahedral sheet. Oa represents the apical oxygen atoms shared with tetrahedra and Ooct is the anionic site shared between adjacent octahedra, a and b (Encyclopaedia Britannica, 1998).
Figure 2.7. The octahedral sites
Figure 2.9. Silicate layer: 1:1 and 2:1 structures
2.5 Influence of Inorganic Acids on Clays
2.6 Clay as a possible Raw Material for Ceramics
Ceramics are solid compounds formed by application of heat, and sometimes heat and pressure, on materials comprising at least two elements provided one is a non-metal or a non-metallic elemental solid. Chemically, with exception of carbon, they are non-metallic inorganic compounds (Barsoum, 2003). Some considerations on physical properties of raw materials for ceramic processing includes fine particle size to provide improved plasticity for forming and higher thermodynamic driving force for sintering and sub micrometer particles that can be more easily packed and mixed in liquids (Murray, 2004). Other properties are ease of deformation without rapture and retention of imposed shape, a relatively non-reactive material that provides a rigid component and a high degree of fineness to make processing easy and give smooth finish (Disdane, 1986). Clays are fine grained in natural state and are aluminosilicates hence meets all the requirements for a raw material for ceramics. It is also naturally-occurring and provides a cheap raw material (Murray, 2002). It is however impure in natural state and require further purification.
2.7 Clay as a Source of Aluminium
Al in Korea and USA where non-bauxite aluminium bearing minerals like kaolin were used. The ore was calcined to 600 oC for two hours and then leached with concentrated hydrochloric acid at 105 oC for one hour. The resulting solution contains both Fe and Al and was subjected to a further purification where Fe was removed by solvent extraction. An aluminium value in the liquor was recovered as AlCl3 hexahydrate, AlCl3.6H2O by crystallisation. The chloride was then thermally decomposed and calcined at 110 oC to produce alumina (Kyun et al., 1979).
Some of the properties of alumina that suit it for use in the clay products are its high melting point, resistance to chemical attack and desirable electrical and mechanical properties. These properties qualify alumina for use in making clay products like refractory components, crucibles, spark plugs, and substrates in electronic devices (Disdane, 1986)
2.7 Effect of Impurities on Properties of Clay
2.7.1 Effect of Silica
Silica occurs in clays as crystalline quartz or in amorphous form. Silica reduces plasticity, drying and firing shrinkage; it reduces firing strength, refractoriness and also causes increase in thermal expansion (Lawrence and West, 1982).
2.7.2 Effect of Alumina
Combined alumina occurs in feldspars, mica, hornblende, tourmaline, bauxite, laterite, diaspore and the clay minerals. When in accessory minerals, alumina reduces plasticity and increases refractoriness (Lawrence and West, 1982).
2.7.3 Effect of Alkalies
The principal alkali-bearing minerals are feldspars, micas and hydrous micas. They could also be present as adsorbed ions on the surface of clay minerals or in form of soluble chlorides and sulphates. Alkalies have strong fluxing action and reduce refractoriness, vitrification temperature and plasticity of clays. They on the other hand impose increase in glass formation which in turn increases the strength of the fired body (Lawrence and West, 1982). Presence of soluble alkalies in clays cause scum formation with soap. Lime is unstable in the atmosphere and takes water thereby causing swelling and breakage of fired product (Daniel, 1972)
2.7.4 Effect of Iron Compounds
reactions which lead to colour changes and glazing temperatures. Fe3O4 in combination with silica starts glass formation at temperatures of 1455 oC. If it gets reduced to FeO, then glass formation can start at a much lower temperature of 1180 oC. Fe2O3 and FeO are brick red and black, respectively, and confer these colours on clay products (Lawrence and West, 1982).
2.7.5 Effect of Calcium Compounds
The calcium compounds found in clays include calcite, aragonite, CaCO3 and gypsum CaSO4.2H2O which decompose on heating to form CaO which acts as a flux. This then results in glass formation and lowers vitrification temperature. It increases the fired strength and reduces absorption of the product. CaO combines with iron minerals and bleaches the red colour to buff. If not fired to sufficiently high temperatures, CaO may remain as free lime which react with water after firing to form Ca(OH)2 which causes large expansion and may develop sufficient pressure to disrupt the fired product (lime popping) (Lawrence and West, 1982).
2.7.6 Effect of Carbonaceous Compounds
2.8 Uses and Applications of Clay and its Minerals
Different clay minerals have different alumina octahedral and silica tetrahedral sheets which cause difference in physical and chemical properties hence differences in the ultimate applications. Particle size, shape and distribution, surface chemistry, area and charge, pH, plasticity, green, dry and fired strength, fired colour, refractoriness, colour and brightness determine the properties and ultimate use of clays (Murray, 2006). Other properties which qualify some clay minerals (more specifically Kaolin) are chemical inertness, white or near white colour, good covering and binding power, softness and non-abrasion, low conductivity of heat and electricity, low viscosity and ability to flow and ability to disperse readily.
2.8.1 Use of Clay in Ceramic Products
past one another. As a result, clay is easily molded into shapes. High temperatures drive out water and allow bonds to form between plates, holding them in place and promoting the formation of a hard solid. Binders such as bone ash are sometimes added to the clay to promote strong bond formation, which makes the ceramic resistant to breakage. The common clay used to make flowerpots and roof tiles is usually red-orange because of the presence of iron oxides. White ceramics are made from rarer (and thus more expensive) white clays, primarily kaolin (Ball and Philip, 1997). Clay is used in manufacture of ceramic products like white ware, tiles, sanitary ware.
2.8.2 Use of Clay in Paper Industry
Clay is used as filler and a coating in the paper industry. As filler, Kaolin is mixed with pulp fibres to form a coating. Kaolin is mixed with water, adhesive and other additives and coated onto the surface of paper. It improves the opacity of the paper sheet, imparts smoothness to the surface and replaces some of the more expensive pulp fibres. As a coating, Kaolin imparts opacity, brightness, a glossy finish, smoothness and improved printing quality (Murray, 2004).
2.8.3 Use of Clay in Paints
viscosity so as to prevent the pigment from settling during storage, provides thixotropy so that the paint is easily applied yet does not sag or run after application, improves gloss, promotes film strength and aid in tint retention (Murray, 2004).
2.8.4 Use of Clay in Plastic and Rubber Industries
Kaolin is the only clay type used in plastic and rubber industries. It is used as an extender and functional filler. Calcined metal-kaolin is used in PVC wire insulator because it enhances electrical resistivity of the wire coating (Sekutowski, 1992).
2.8.5 Use of Clays in Inks
Kaolins are ingredients of printing ink where they act as extenders of the polymer present in ink, improve colour intensity, limit ink penetration into paper, control rheology and improve adhesion (Murray, 2004).
2.8.6 Use of Clay as Cracking Catalyst
2.8.7 Clay as a Chemical Raw Material
Air-floated kaolin is used as a chemical raw material to make fiberglass. Kaolin is also used in some cement plants to whiten the colour and to provide silica and alumina for cement reactions, and increase cement strength. Kaolin is used as a raw material for producing zeolites which are an ingredient in detergent (Murray, 2006).
2.8.8 Use of Clay in Pencil Leads
Kaolin is used as an additive to graphite in making pencil leads. Plasticity and fine particle nature of kaolin are useful in extruding the graphite-kaolin mixtures (Murray, 1961).
2.8.9 Use of Clays in Suspensions and Diluents
Kaolins are used as suspending agents in pharmaceuticals, cosmetics, enamels and medicines. Some pills use kaolin as a diluents and a binder in pressing pills (Murray, 2004).
2.8.10 Use of Clays in Fertilizers, Desiccants and Insecticides
2.8.11 Use of Clay in Roofing Granules and Polishing Compounds
Roofing granules are produced by calcining coarse granular particles of white kaolin. Fine particle calcined kaolin of 3 µm is used in polishing compounds for automobiles, silver, copper, brass and other metals (Murray, 2004).
2.8.12 Use of Clay as Drilling Mud
Sodium montmorillonite is the major constituent of high swelling clays. The high-swelling property makes the clay a necessary ingredient in fresh water drilling muds in the world. Only 5% by weight of the high-swelling clay are required to produce the high viscosity, thixotropic fluid with low filter cake permeability necessary to meet the American Petroleum Institute (API) drilling fluid specifications (Murray, 2004).
2.9 Analytical Methods/Instruments
2.9.1 Atomic Absorption Spectrometry (AAS) analysis
188.8.131.52 Instrumentation of AAS
AAS instrument has four main parts namely, the hollow cathode lamp, the flame atomizer, the spectrometer and the signal read out. The hollow cathode lamp is the radiation source. It is cylindrical with a metal of choice as cathode or anode, and filled with argon or neon gas. A high voltage is applied across the cathode and anode to ionize the gas particles inside. As the voltage is increased, the ionized gas particles acquire enough energy to eject metal atoms from the cathode. Some of the ejected atoms are in an excited state and emit light with characteristic frequency to the metal under investigation. The sample is first dissolved and nebulized/aspired into the flame which vaporizes it and frees it from the atoms/ions of all the other elements present ( Alkemade et al., 1982; L’vov, 2005).
184.108.40.206 Working Principle of AAS
Where; A = absorbance (No units), b = path length (cm), c = molar concentration (mol dm-3), ε = molar absorptivity (dm3 mol-1 cm-1). Calibration is done such that a given absorbance gives a corresponding concentration.
2.9.2 X-Ray Diffraction (XRD) Analysis
XRD is a versatile non-destructive analytical technique that reveals detailed information about the chemical composition and crystallographic structure of natural and manufactured materials. It is a rapid analytical technique used primarily for phase identification of crystalline materials and can provide information on unit cell dimensions. XRD is the basic analytical tool used for identification and characterization of clay minerals (Brindley and Brown, 1981).
220.127.116.11 Principle of XRD
radiation (Figure 2.10), (Harris and White, 2007). These X-rays are generated by a cathode ray tube, filtered to produce monochromatic radiation, collimated to concentrate, and directed toward the sample. The interaction of the incident rays with the sample produces constructive interference (and a diffracted ray) when conditions satisfy Bragg's Law (nλ=2d sin θ). This law relates the wavelength λ, of electromagnetic radiation to the diffraction angle θ and the lattice spacing d in a crystalline sample. These diffracted X-rays are then detected, processed and counted. By scanning the sample through a range of 2 θ angles, all possible diffraction directions of the lattice should be attained due to the random orientation of the powdered material. Conversion of the diffraction peaks to spacings allows identification of the mineral because each mineral has a set of unique d-spacings. Typically, this is achieved by comparison of d-spacings with standard reference patterns (Moecher, 2004). The crystalline substances act as three dimensional diffractions gratings for X-ray wavelengths similar to the spacing of planes in a crystal lattice (Max von Lane, 1912). A crystal lattice is a regular 3-dimentional distribution of atoms in space with atoms arranged such that they form parallel planes separated by a distance d, which varies according to the nature of the material. Spectral peaks are produced which give the identity and intensity of the clay minerals (Chipera and Bish, 2001).
18.104.22.168 Instrumentation and Working of XRD
electrons which are then accelerated towards the target material by applying a voltage difference. The accelerated electrons bombard the target material and dislodge inner shell electrons thereby creating a vacuum. Electrons from higher energy levels then release energy and occupy void lower energy level and cause production of characteristic x-ray spectra. The spectra produced comprises of several components, the most common being Kα and Kβ (Figure 2.10).
Figure 2.10 (A) Schematic of an atom, depicting electron shells and the energy transitions for Kα, Kβ, and Lα characteristic radiation. (B) Generalized depiction of an X-ray spectrum, showing peaks in intensity at wavelengths (energy levels) corresponding to char-acteristic radiation.
directed into the sample. As the sample and detector are rotated, the intensity of the reflected x-rays is recorded and peak intensity is recorded when the geometry of the incident x-rays impinging the sample satisfies Bragg’s equation and constructive interference occurs. The peak signal is recorded by the detector, processed and converted into a count rate which is then printed in the output device or computer. The geometry of an x-ray diffractometer is such that the sample rotates in the path of collimated x-ray beam at angle θ while the x-ray detector rotates at angle 2θ.
2.9.3 Infrared Spectroscopy (IR)
22.214.171.124 Principle of Infrared Spectroscopy (IR)
is used to determine the concentration of the sample according to Lambert’s law, I = Io exp (-εcl),
where, I = the intensity of incident radiation, Io = intensity of emitted radiation, l = length of the sample, c = concentration of the specimen,
ε = constant characteristic with the transition
For identification of the minerals in clays, the infrared spectrum of the sample is used. The infrared spectrum for each mineral is characteristic and different from that of the other (Wilson, 1996).
126.96.36.199Instrumentation in IR
Infrared spectrophotometers have three basic parts which comprises of the source of radiation which is commonly an inert solid body which is heated electrically to temperatures between 1500 oC and 2000 oC, the monochromator for dispersing the radiation and the detector which registers the residual intensity after selective absorption by the sample.
2.9.4 Ethylenediaminetetraacetic Acid (EDTA) Titration`
MATERIALS AND METHODS 3.1 The Study Area
Kano plains are located in Kisumu County in the Republic of Kenya. The study area is found between latitude E 34o25’, E 35o50’ and longitude 0o00’ and N 0o24’ and is about 60 km2 as shown in the map in figure 3.1.
Soil map of Kano Plains (Figure 3.2) reveal that the soils are majorly clay of different depths mixed sparingly with loams and a few areas with sandy soils. This is supported by physical clay characteristics of the soils such as plasticity when wet, poor drainage which partly lead to flooding due inability to absorb water leading to surface run-off, hardening and cracking of the soils during dry seasons.
Table 3.1. The sampling sites and sample indexing
S/No. Sample No. Sampling Site Grid Reference 1 3076 Nyaidho River Bank(Oren) E 35o05’, S 0o11’ 2 3077 Chiga Kolwa Village E 34o52’, S 0o07’ 3 3078 Thurgem Secondary School E 35o01’, S 0o18’ 4 3079 Riat Market E 34o51’, S 0o15’ 5 3087 Karanda Primary School E 34o70’, S 0o11’
6 3098 Okana Site E 34o50’, S 0o08’
7 3100 Anywang’ River bank E 34o50’, S 0o05’ 8 3104 Kobura Rice Scheme E 34o75’, S 0o10’
3.2 Apparatus, Chemicals and Materials
All apparatus and chemicals used were of analytical grade and had the standard specifications for the analyses. Specifications of additional apparatus and instruments used include;
i) Jenway pH meter, Model 3510 manufactured in UK
ii) Sartorius top pan electronic weighing balance, Supplied by Acheles Kenya, Ltd, Nairobi iii) Atomic Absorption Spectrometer named Spectro AA.10(Varian), Supplied by Labtec
Table 3.2 Percentage mineral composition of rock standards, (CCMET, 1991)
SiO2 Al2O3 Fe2O3 MgO CaO Na2O K2O TiO2 MnO P2O5
SY-2 60.07 12.15 5.92 2.66 8.03 4.37 4.52 0.15 0.33 0.07 MRG 39.09 8.46 17.94 13.55 14.71 0.74 0.18 3.69 0.03 0.09
The instrumental conditions for AAS analysis for different elements were set as indicated in table 3.3.
Table 3.3 Instrumental conditions and settings for AAS analysis (CCMET, 1991)
Element Lamp current(A)
Slit width (nm)
Si 7 0.2 251.6 4.5 359.3 N2
Al 6 0.5 309.3 4.5 287.4 N2
Fe 8 0.2 248.3 1.5 340.5
Ca None 0.5 422.7 4.5 231.1 N2
Mg 3 0.5 285.2 1.5 318.6
Mn 5 0.2 279.5 1.5 349.9
Ti 10 0.5 364.3 4.5 303.0 N2
K None 1.0 766.5 1.5 353.5
Na None 0.5 589.0 1.5 365.5
iv) X-Ray Fluorescence (XRF) spectrometer, Mini Pal 2 supplied by Philips
The voltage and current settings for analysis of different elements are done automatically by the Mini Pal software upon selection of the element Table 3.4).
Calibrations for the analyses are also automated using Rock standard samples.
Table 3.4 XRF voltage and current settings for analysis of elements in clay samples
Element (in oxide form) Voltage setting (kV) Current setting (mA)
SiO and Al2O3 4.09 1.000
Fe2O3 20.00 0.010
MnO 8.00 0.100
v) Infrared Spectroscopy (IRS)FTIR-8400 model Supplied by Shimadzu, Japan was used. Mini hand press Model MHP-1 was used to prepare pellet discs. Polystyrene mortar and pestle were used to mix and grind clay and KBr into powder. Chemical balance model AUY 220 from Shimadzu Corporation Japan was used in weighing clay samples and KBr.
vi) X-ray diffractometer Model D2Phaser supplied by Bruker was used. Settings were 2θ, Cu operated at a voltage and current of 40 kV and 30 mA respectively.
vii) Pulveriser: Name: SIEBTECHNIK, Model: TEMA B.V, Model T 5250 Jaw crusher Supplied by Denver, England.
ix) Pelleting machine Herzog, Type TP 2 OP Mazchinenfabric + Co, D – 49086 Osnabruck –Germany
3.3 Sample Pre-Treatment and Analysis 3.3.1 Drying and Grinding Of the Samples
The samples were transferred into clean glass beakers, dried in the oven at 105 ºC for six hours and then cooled in a dessicator. The dried samples were fed into the primary crusher and then secondary crushers of the Siebtechnik model T 5250 ball mill steel mortar and ground into powder sizes suitable for use in XRD, XRF instruments, and digestion by inorganic acids for subsequent laboratory analyses (Norton, 1974, Richerson, 1992).
3.3.2 Digestion for AAS Analysis
in a clean automatic liquid dispenser and diluted to 100.0 ml in 100 ml volumetric flask in readiness for AAS analysis.
3.3.3 Pelleting for XRF Analysis
Oven dried clay powder of 10.0 g was accurately weighed in an electronic weighing balance and transferred into a clean dry porcelain crucible. Five grammes of starch powder was weighed and added to the sample. The mixture was ground and uniformly mixed into a fine powder using the pestle and then transferred into the pellet binder. The clay-starch mixture was placed into a compressor and compressed to 175 kN to form clay pellets. The pellets were then labelled and analysed for mineral composition.
3.3.4 Preparation of Alkali Halide Pressed Discs for IR Analysis
About 2.0 mg of dry powdered clay was mixed with about 170 mg of KBr crystals and ground for about 2 minutes in a polystyrene mortar with a pestle. The powdered mixture was fed into the “Mini hand press” and compressed into a disc. The disc was then placed in the sample holder of the IR spectrometer for mineral analysis.
3.3.5 Preparation for EDTA Titrations 188.8.131.52 Preparation of 0.05 M EDTA Solution
shaken to dissolve the crystals. More water was added to the mark and mixture shaken for homogeneity.
184.108.40.206 Preparation of Solochrome Black (Eriochrome Black T) Indicator
Accurately weighed dyestuff of mass 0.2 g was added to 15.0 cm3 of triethanolamine and the mixture stirred to dissolve. A portion of 5.0 cm3 absolute ethanol was then added to the mixture to reduce viscosity (Mendham et al., 1989).
220.127.116.11 Preparation of 0.01 M Zinc Sulphate Solution
Hydrated zinc sulphate crystal weighing 2.8754 g was transferred into a clean I Litre volumetric flask. Distilled water was then added in portions with shaking till all the crystals dissolved. More distilled water was added to the mark and the mixture shaken for homogeneity (Mendham et al., 1989).
18.104.22.168 Preparation of Standard 0.05 M Fe3+ Solution
3.3.6 Determination of Fe3+ and Al3+ In Raw and Acid-Treated Clays By EDTA Titration
22.214.171.124 Determination of Fe3+ in clay samples by EDTA titration
Using a pipette, 25 cm3 portions of digested clay solution was placed in a conical flask and diluted to 100 cm3 using de-ionized water. The pH was adjusted to 2-3 using ammonium hydroxide solution and hydrochloric acid complementarily. 5 drops of Variamine blue indicator was added and the mixture warmed to 40 oC. The solution was then titrated with approximately 0.05 M- EDTA solution till the blue colour turned grey just before turning yellow at the end-point. The experiment was done in triplicate and average titre used to determine the moles and later amount of Fe in the sample. [1 mole EDTA = 1 mole Fe3+]. (Mendham et al., 1989).
126.96.36.199 Determination of Al3+ In Clay Samples by EDTA Titration
added from a burette used in the back-titration corresponds to 0.2698 mg Al] (Mendham
et al., 1989).
3.4 X-Ray Fluorescence Spectrophotometer (XRFS) Analysis
The prepared clay pellets were fed in the sample holders in the XRF spectrometer. The setting for “application analysis” mode was selected from default program in the Mini Pal software and the element of choice selected. The software has default calibrations for a given element analysed and the analysis proceeds automatically on the press of a button. The percentage composition of the element in oxide form is displayed on the screen. The procedure as repeated for the other elements on test and the results recorded. The application mode was used for analysis.
NB: The analysis for Fe was done based on “Ferric oxide” calibrations, while that for Al was done using the “Alumina” calibrations.
3.5 X-Ray Diffraction (XRD) Analysis
per step. The diffractometer produced signals on a screen and the names and formulae of the minerals printed. Clay mineral diffraction patterns contain a good deal of character. This character is manifested by the peak’s position, intensity, shape, and breadth. Peak position is determined by the Bragg law which is written as nλ = 2dsinθ. If the analysis is
one dimensional, l may be substituted for n and the equation rearranged to give lλ/2d = sinθ. Now we have two constants, d = d(001) and λ, and if θ is small, the angle may be
Table 3.5 Major d-spacings for some minerals that occur in soils, listed for each mineral in the commonly observed order of decreasing XRD peak intensity.
Mineral groups Minerals Major d-spacings
Å Expansible phyllosilicates Montmorillonite 18.0, 9.0, 4.49
Vermiculite 14.4, 7.18, 4.79, 3.60 Feldspars Albite 3.19, 4.03, 3.21
Anorthite 3.20, 3.18, 4.04 Microcline 3.24, 3.29, 4.22 Orthoclase 3.31, 3.77, 4.22
Kaolins Halloysite 10.7–10.0 (Hydrated), 7.6, 4.4, 3.4
Kaolinite 7.17, 3.58,
Micas Biotite 10.1, 3.37, 2.06
Muscovite 10.1, 3.36, 5.04 Oxides, hydroxides Anatase 3.51, 1.89, 2.38 Gibbsite 4.85, 4.37, 2.39 Goethite 4.18, 2.45, 2.70 Hematite 2.69, 2.59, 1.69 Ilmenite 2.74, 2.52, 1.72 Quartz 3.34, 4.26, 1.82 Rutile 3.26, 1.69, 2.49 Zeolites and related
3.43, 5.60, 2.93
Palygorskite 10.4, 4.47, 4.26 Sepiolite 12.1, 2.56, 4.31
3.6 Infrared (IR) Analysis
The wavenumbers from the spectrum are then used to identify the corresponding minerals.
The appearance of ν (Si–O–Si) andδ (Si–O) bands also support the presence of quartz (Marel and Bentelspacher, 1976) a strong band at 3696⋅7 cm–1,3622⋅5 cm–1 and 3450⋅4 cm–1 indicate the possibility of the hydroxyl linkage. However, a broad band at 3450⋅4 cm–1 and a band at 1633⋅4 cm–1 in the spectrum of clay suggest the possibility of water of hydration in the adsorbent. The inter-layer hydrogen bonding in clay is assigned by a characteristics band at 3622⋅5 cm–1. Most of the bands such as 3696⋅7 cm–1, 3622⋅5 cm–1, 3450⋅4 cm–1, 1033⋅3 cm–1, 914⋅5 cm–1, 790⋅9 cm–1, 693⋅4 cm–1, 538⋅8 cm–1, 468⋅9 cm–1 show the presence of kaolinite (Tuddenham and Lyon, 1960). The vibrations observed at 914⋅5 cm–1 indicate the possibility of the presence of hematite (Gadsen, 1975). The presence of bands at 3696⋅7 cm–1, 3622⋅5 cm–1, 3450⋅4 cm–1, 2369⋅8 cm–1, 1633⋅4 cm–1, 1033⋅3 cm–1, 914⋅5 cm–1 and 790⋅9 cm–1
indicate the possibility of the presence of illite (Wolf, 1963), whereas 3622⋅5 cm–1, 1633⋅4 cm–1, 1033⋅3 cm–1
are indicative of gypsum and 693⋅4 cm–1 shows the possibility of the presence of calcite (Gadsen, 1975). The corresponding values are given in table 4. Thus the results of IR are quite helpful in the identification of various forms of minerals present in the used sorbents. IR spectra of these sorbents show adsorption band at 3622⋅5 cm–1 of clay corresponding to H
Table 3.6 IR Identification peaks for clay minerals
Mineral Identification Peaks (cm-1)
Kaolinite 3696, 3670, 3654, 3620, 3440, 1111, 1032, 1009, 913, 794, 754, 698, 538, 470, 431 cm-1
Illite 3621, 3340, 3625, 3421, 1024, 912, 829, 799, 750, 527, 471, 434 cm-1 Montmorillonite 3626, 3424, 3419, 1634, 1039, 915, 843, 796, 623, 522, 466 cm-1
Muscovite 3624, 3621, 3435, 3431, 1026, 912, 820, 790, 753, 632, 629, 474, 417 cm-1 Chlorite 3548, 3424, 1628, 985, 758, 649, 548, 453, 435 cm-1
Feldspar 1146, 1090, 1034, 1011, 780,693, 688, 533, 464, 428 cm-1
Calcite 2672, 2513, 1719, 1422, 876, 711 cm-1
Quartz 1871, 1171, 1082, 796, 779, 695, 514, 460 cm-1
IR spectra have been published by( Moenke, 1962; Van der Marel and Beutelspacher, 1976; Ferraro, 1982; Kodama 1985).
then dried in the oven at 105 oC for six hours, cooled to room temperature and then subjected to analysis of residual Fe, Si and Al using AAS, XRF and EDTA titrations (For Fe and Al only). The percentage composition of the elements, expressed as oxides were recorded in tables and graphs. Physical factors of the clay like particle size, clay-acid ratio and duration of leaching were kept constant. The room temperatures of 25oC were also kept constant.
3.8 Loss On Ignition (LOI)
Powdered, dry clay sample of 0.10 g, accurately weighed was placed in a porcelain crucible and heated to 1000 oC in a furnace for one hour. It was then placed in a
RESULTS AND DISCUSSION 4.1 Introduction
The findings from elemental and mineral analytical procedures are presented in tables, diagrams and and graphs. Detailed results and findings are found in the appendices. The elemental compositions are expressed in percentage of oxides of the respective elements for raw and acid-treated clays as given by AAS and XRF. For the acid-treated clays, elemental compositions of the three major minerals, silica, alumina and iron(iii) oxide are given for residual clay after acid treatment since special interest was to determine levels of iron in clays after acid-treatment. For mineral analysis, the name, formulae and percentage composition of minerals are given as determined by XRD for both raw and acid-treated samples. The IR analysis results are presented by spectra for selected samples. The spectra of peaks of identified minerals are shown together with a summary of percentage composition and elemental constitution of individual minerals.
4.2 Chemical Analysis of Raw Clays in the Study Kano Plains
Table 4.1 Full Assay analysis of clays from Kano Plains by AAS with percentage composition of elements expressed in oxide form
Sample SiO2 Al2O3 Fe2O3 K2O Na2O TiO2 CaO MgO MnO LOI TOTAL
3076 62.37±0.02 14.33±0.45 4.33±0.11 3.11±0.08 1.86±0.01 1.22±0.01 0.80±0.01 0.45±0.01 0.20±0.01 10.03±0.06 98.76±0.47
3077 64.70±0.10 13.65±0.08 3.74±0.08 2.40±0.05 1.16±0.02 0.92±0.02 0.56±0.02 0.44±0.01 0.02±0.01 10.99±0.10 98.58±0.31
3078 61.44±0.06 12.54±0.37 5.94±0.06 2.84±0.02 1.76±0.01 1.18±0.01 1.04±0.01 0.77±0.01 0.24±0.01 11.00±0.11 98.79±0.43
3079 49.85±0.28 17.21±0.27 10.28±0.06 2.43±0.15
1.08±0.02 2.49±0.01 1.67±0.01 1.12±0.02 0.23±0.01 15.40±0.10 101.75±0.73
3087 45.47±0.18 14.47±0.36 5.94±0.06 2.31±0.02 1.06±0.03 2.01±0.01 1.71±0.02 1.06±0.02 0.21±0.01 14.17±0.15 88.37±0.36
3098 53.37±0.09 16.53±0.30 10.28±0.06 2.07±0.01 0.98±0.01 2.23±0.01 1.69±0.01 1.15±0.02 0.21±0.02 12.67±0.01 101.06±0.23
3100 54.24±0.12 17.95±0.19 5.68±0.10 2.50±0.02 1.35±0.02 1.52±0.01 1.15±0.02 0.73±0.01 0.13±0.01 9.77±0.15 95.01±0.13
Table 4.2 Ranges of percentage elemental composition, as oxides, from Full assay AAS analysis of raw clays from Kano plains
Element(Oxide) Range of percentage composition of oxides
SiO2 45.47±0.18- 64.70±0.10
Al2O3 12.54±0.37- 17.75±0.19 Fe2O3 3.74±0.08- 10.28±0.06 K2O 2.31±0.0.02- 3.11±0.08 Na2O 0.98±0.01- 1.86±0.01
CaO 0.56±0.02- 1.71±0.02
MgO 0.44±0.01- 1.15±0.02
TiO2 0.92±0.02- 2.49±0.01
MnO 0.02±0.01- 0.24±0.01
LOI 9.77±0.15- 15.40±0.10
Table 4.3 Percentage mean composition of different minerals in raw clays by different methods
Element Method Range of % oxide(Site mean) Overall mean SiO2 AAS 45.47±0.18 - 64.70±0.10 55.15±0.26
XRF 47.53±0.23- 65.92±0.04 57.10±1.30 Al2O3 AAS 12.54±0.37 - 17.95±0.19 15.30±0.17 XRF 14.68±0.20 - 19.55±0.30 16.62±0.35 EDTA 13.30±0.10 - 18.57±0.06 15.78±0.38 Fe2O3 AAS 3.74±0.08 - 10.28±0.06 7.00±0.53
XRF 5.18±0.15 - 11.54±0.07 8.63±0.46 EDTA 4.16±0.06 - 10.56±0.08 7.48±0.51 Na2O AAS 0.98±0.01 - 1.86±0.01 1.32±0.01 K2O AAS 2.07±0.01 - 3.11±0.08 2.56±0.07
XRF 2.33±0.02 - 3.41±0.06 2.86±0.07 MgO AAS 0.44±0.01 - 1.17±0.02 0.86±0.01 MnO2 AAS 0.20±0.01 - 0.25±0.01 0.19±0.01
XRF 0.05±0.00 - 0.19±0.01 0.14±0.01 TiO2 AAS 0.92±0.02 - 2.35±0.01 1.74±0.02 XRF 0.77±0.01 - 2.23±0.01 1.50±0.11 CaO AAS 0.56±0.02 - 2.34±0.01 1.37±0.05
XRF 1.18±0.00 - 2.84±0.02 1.93±0.12
The results obtained from XRF gave elemental compositions of almost same ranges but are consistently slightly above those obtained from AAS analyses because of strong and severe X-ray absorption and enhancement effects in XRF but not in AAS (Brundle et al., 1992). EDTA titration analyses were only done for Fe3+ and Al3+. The percentage compositions from EDTA analysis were slightly above measurements from AAS but slightly below the measurements from XRF as shown in table 4.3.
4.3 Mineral Analysis of Raw Clays 4.3.1 XRD Analysis of Raw clays
4.3.2 IR Analysis of Raw Clays
The IR bands found in the clay minerals from Kano plains range from about 3700cm-1 to 470cm-1. The peaks at 3695, 3668, 3652, 3620 cm-1 are stretching inner bands of -OH groups characteristic of kaolinite. Other peaks that support presence of kaolinite are found at 1635.5 cm-1 which is deformation band of water for kaolinite, illite and montmorillonite, and 1100 cm-1, Si-O stretching and 528.5 cm-1, Al-O-Si deformation band of kaolinite. The IRS also indicate presence of montmorillonite evidenced by peaks at 1010-1030 cm-1, In-plane Si-O stretching band, 935cm-1, deformation Al-Al-O vibrational band, 820 and 757 cm-1 tetrahedral Al–O out-of-plane and Al–O–Si in-plane vibrations respectively, and 625 cm-1 , coupled out-of-plane vibrational band of Al-O and Si-O. Other minerals found in the clays are illite and biotite. Illite is identified by the peaks at 3606.6 cm-1, stretching band of structural hydroxyl groups (both illite and biotite), 3436.9 cm-1 , stretching bond of water, and 1635.5 cm-1, deformation band of water (Illite, kaolinite, montmorillonite).
dominate the 150-600 cm-1 region. Lattice vibrational modes in the far-IR range (33 - 333 cm-1) are related to the interlayer cations (Schroeder, 2002). Some peaks observed during IR analysis of clays from Kano plains are shown in figures 4.2(a) and (b).
Table 4. 4 The IR peaks identified, deformation assignments and corresponding minerals in clays of Kano planes
Peaks/Bands (cm-1) Deformation assignment Characteristic
3436.9 (Sample 3077, 3079) 1635.5 (All samples)
1010-1030 cm -1 (3079, 3098, 3078)
902.6 (Samples 3076, 3077)
820 and 757 cm -1 (3100, 3078,3076)
528.5 (Sample 3076, 3079, 3100) 466.7 (Sample 3076, 3078, 3100)
Stretching bands of inner OH groups Stretching band of structural hydroxyl groups
Stretching bond of water Deformation band of water
Si-O stretching band
In-plane Si-O stretching band Deformation Al-Al-O vib. band Stretching Si-O band
Coupled out-of-plane vib. band of Al-O and Si-O
Tetrahedral Al–O out of plane and Al– O–Si in plane vibrations respectively Deformation band of Al-O-Si
Deformation band of Si-O-Si
Kaolininte, illite, montmorillonite Kaolinite
4.4 Chemical Analysis of Acid-Treated Clays
Acid treatment causes a reduction in composition of most elements with a higher reduction being achieved at higher concentrations and temperatures. The boiling temperature of acid-clay mixture varied differently with concentrations for HCl and H2SO4 (Table 4.5). The acid-clay mixture boiling temperature for HCl increases from 97oC at 2M acid concentration to a maximum of 105oC at 8M concentration and then reduces to about 76oC at 11 M acid concentration due to higher volatility of the acid in the mixture at higher concentrations. For the less volatile H2SO4 the acid-clay mixture boiling temperature increases steadily from 99oC at 2 M to about 310oC at 18 M acid concentration.
Table 4.5 Boiling temperature of Acid-clay mixtures for HCl and H2SO4 at different acid
Acid concentration (Mol/L) 2 4 6 8 10 11 18 Boiling temperature of HCl-clay
97 100 104 105 98 76 Boiling temperature of H2SO4-clay
99 103 112 125 165 310
4.4.1 Treatment with Different Concentrations of HCl and H2SO4 at Room Temperature (25oC)
dependent. This is likely due to absence of iron in the mineral structure as evidenced from mineral analysis.
There was however no appreciable change in percentage composition of Al and Si and this was likely due to the presence of the elements in the mineral structure of the clays. The non-effect of composition of Si is due to both its being a structural component of the minerals and insolubility in mineral acids which cause increase in its percentage as the other elements dissolve (Table 4.6).
Table 4.6 Percentage SiO2, Al2O3 and Fe2O3 in HCl-treated clays at room and boiling temperatures
Element (In oxide form)
Raw 2M 4M 6M 8M 10M 11M
Fe2O3 % at 25oC 8.25 6.76 6.13 5.78 4.63 4.19 3.12
% at Boiling Temperature
8.25 5.33 3.11 1.74 1.45 2.01 1.58 Al2O3 % at 25oC 15.90 14.20 15.51 14.59 14.42 13.70 15.37
% at Boiling Temperature
15.90 13.68 12.47 12.24 14.24 13.22 12.52 SiO2 % at 25oC 55.15 55.27 55.31 56.38 57.54 55.56 55.20
% at Boiling Temperature
4.4.2 Treatment with Different Concentrations of HCl and H2SO4 at Boiling Temperatures